- Nano Express
- Open Access
A New Up-conversion Material of Ho3+-Yb3+-Mg2+ Tri-doped TiO2 and Its Applications to Perovskite Solar Cells
Nanoscale Research Lettersvolume 13, Article number: 262 (2018)
A new up-conversion nanomaterial of Ho3+-Yb3+-Mg2+ tri-doped TiO2 (UC-Mg-TiO2) was designed and synthesized with a sol-gel method. The UC-Mg-TiO2 presented enhanced up-conversion fluorescence by an addition of Mg2+. The UC-Mg-TiO2 was utilized to fabricate perovskite solar cells by forming a thin layer on the electron transfer layer. The results display that the power conversion efficiency of the solar cells based on the electron transfer layer with UC-Mg-TiO2 is improved to 16.3 from 15.2% for those without UC-Mg-TiO2. It is demonstrated that the synthesized UC-Mg-TiO2 can convert the near-infrared light to visible light that perovskite film can absorb to improve the power conversion efficiency of the devices.
More attentions have been paid to the perovskite solar cells (PSCs) in the field of solar cells [1,2,3,4,5]. The power conversion efficiency (PCE) of the PSCs has been exceeding 22% within a few years . However, the perovskite materials usually absorb the visible light whose wavelength is less than 800 nm, and more than half of the solar energy is not be utilized, especially in the region of near-infrared (NIR). To solve the issues, one of the effective methods is to apply the up-conversion nanomaterial to perovskite solar cells by converting the NIR light to visible light that the perovskite can utilize [7,8,9]. The beta-phase sodium yttrium fluoride (β-NaYF4) is commonly used as the host lattice for rare earth ions to prepare the up-conversion materials. While the β-NaYF4-based up-conversion materials are insulator, which is not beneficial for the electron transfer [ETL] .
Titanium dioxide (TiO2) nanocrystal with anatase phase is commonly used as the electron transfer material in the perovskite solar cells due to its suitable energy band structure, low cost, and long stability [11,12,13]. However, the energy band gap of TiO2 is large (3.2 eV), which hampers its applications. To improve the applications of TiO2 in visible light and near-infrared region, some methods were explored. One of the effective methods is doping TiO2 with metal or non-metal [14,15,16]. Yu et al.  demonstrated that Ho3+-Yb3+-F− doped TiO2 could convert NIR light to visible light that can be absorbed by the dye-sensitized solar cells (DSSCs). Zhang and co-authors  proved that Mg-doped TiO2 can change the Fermi energy level of TiO2 to enhance the performance of perovskite solar cells.
In this work, we are preferred to combine the rear earth ions (Ho3+ and Yb3+) and the metal ion (Mg2+) doped TiO2 together to synthesize a new material with enhanced up-conversion fluorescence. Our purpose is to explore how the addition of Mg2+ affect the up-conversion fluorescence of TiO2 and to apply the up-conversion nanomaterial of Ho3+-Yb3+-Mg2+ tri-doped TiO2 to perovskite solar cells. The results display that the addition of Mg2+ enhanced the up-conversion emission of TiO2, and the application of Ho3+-Yb3+-Mg2+ tri-doped TiO2 improved the PCE of PSCs to 16.3% from 15.2%.
Formamidinium iodide (FAI), Methylamium bromide (MABr), Lead diiodide (PbI2), 2,2′,7,7′-Tetrakis-(N,N-di-p-methoxyphenylamine)-9,9′-spirobifluorene (Spiro-OMeTAD), and lead dibromide (PbBr2) were purchased from Xi’an Polymer Light Technology Corp. (China). The SnO2 colloid solution was purchased from Alfa Aesar (tin (IV) oxide). Dimethyl sulfoxide (DMSO), N,N-dimethylformamide (DMF), 4-tert-butylpyridine (TBP), and lithium bis (trifluoromethanesulfonyl) imide (Li-TFSI) were purchased from Shanghai Aladdin Bio-Chem Technology Co., LTD (China).
Synthesis of Ho3+-Yb3+-Mg2+ Tri-doped TiO2
The up-conversion material of Ho3+-Yb3+-Mg2+ tri-doped TiO2 was synthesized with a reported method  with some modifications. Firstly, a Titanium tetrabutanolate was obtained by mixing acetylacetone (AcAc) and Titanium tetrabutanolate (Ti(OBu)4) for 1 h under stirring at 25 °C, and then the isopropyl alcohol (IPA) was added to prepare the (Ti(OBu)4) solution. A mixed solution of IPA, HNO3, and H2O was dropped into the solutions slowly. After stirring for 6 h, a TiO2 sol with a color of light yellow was obtained. In a typical synthesis, the molar ratio of AcAc, HNO3, and H2O to Ti(OBu)4 was 1:0.3:2:1. For the synthesis of Ho3+-Yb3+ co-doped TiO2, Ho(NO3)3·5H2O and Yb(NO3)3·5H2O were used as the elemental sources and added into the solution. Typically, the molar ratio of Ho3+:Yb3+:Ti = 1:x:100 (x = 2, 3, 4, 5). For the synthesis of Ho3+-Yb3+-Mg2+ tri-doped TiO2, Ho(NO3)3·5H2O, Yb(NO3)3·5H2O, and Mg(NO3)2 6H2O as the elemental sources were added into the solution, and the molar ratio of Ho3+:Yb3+:Mg2+:Ti = 1:4:x:100 (x = 0, 1, 1.5, 2, 2.5). The obtained solution was referred to as Ho3+-Yb3+-Mg2+ tri-doped TiO2 (UC-Mg-TiO2) sol. The solvent in the solution was removed by heating at 100 °C for 10 h. Then, the material powders were heated for 30 min at 500 °C.
Preparation of PSCs
The FTO was washed in detergent, acetone, and isopropanol, and then treated for 15 min with UV-O3. A blocking layer was prepared by a spin-coating method using a solution of titanium diisopropoxide bis (acetylacetonate) in 1-butanol with the concentration of 1 M and then heated for 30 min at 500 °C. An electron transfer layer (ETL) prepared by a spin-coating method using TiO2 solution which is obtained by diluting TiO2 (30NR-D) using ethanol (1:6, mass ratio), and then heated for 10 min at 100 °C and 30 min at 450 °C. The UC-Mg-TiO2 was used to fabricate the solar cells by spin-coating a mixed solution of UC-Mg-TiO2 sol and TiO2 sol (UC-Mg-TiO2:TiO2 = x:(100 − x), v/v, x = 0, 20, 40, 60, 80, and 100) on the ETL and heating for 30 min at 500 °C. A perovskite film was fabricated according to the reported method . In brief, the precursor solution of perovskite was prepared by dissolving FAI (1 M), PbI2 (1.1 M), MABr (0.2 M), and PbBr2 (0.22 M) in the mixture of DMF/DMSO (4:1 v:v), and a stock solution of CsI (1.5 M) in DMSO was added. The perovskite film was obtained by spin-coating method with 1000 rpm for 10 s and 4000 rpm for 30 s, and 200 μL chlorobenzene was dropped on the sample before the end of 20 s. A hole transfer layer (HTL) was obtained by the spin-coating method using a spiro-MeOTAD solution at 4000 rpm for 30 s. The spiro-OMeTAD solution was prepared by dissolving 72.3 mg spiro-MeOTAD in 1 mL chlorobenzene and by adding 28.8 μL TBP, 17.5 μL Li-TFSI solution (520 mg/ml in acetonitrile). Finally, an Au anode was made on the hole transfer layer by thermal evaporation.
Photoluminescence (PL) spectra were acquired using a fluorometer of FLS 980 E. A diffractometer of DX-2700 was used to obtain the X-ray diffraction (XRD) patterns. X-ray photoelectron spectra were measured with a spectrometer of XPS THS-103. Absorption spectra were obtained with a spectrophotometer of Varian Cary 5000. Scanning electron microscope (SEM) images were performed using a microscope of JSM-7001F. A Keithley 2440 Sourcemeter was applied to measure the photocurrent-voltage (I-V) curves of the solar cells under an illumination of AM 1.5. An electrochemical workstation of CHI660e was utilized to get the electrochemical impedance spectroscopy (EIS). The incident photon-to-current conversion efficiency (IPCE) was measured with a solar cell IPCE recording system (Crowntech Qtest Station 500ADX).
Results and Discussion
The up-conversion fluorescence of the materials was optimized by varying the molar ratio of Ho3+ and Yb3+. The up-conversion emission of Ho3+-Yb3+ co-doped TiO2 with varying molar ratio of Ho3+ and Yb3+ (Ho:Yb:Ti = 1:x:100) was shown in Fig. 1a, which were excited with an 980 nm NIR light. Two strong up-conversion emission peaks were observed at 547 nm and 663 nm. Additional file 1: Figure S1 shows the up-conversion mechanisms of the Ho3+-Yb3+ co-doped TiO2. The fluorescence peaks at 663 nm and 547 nm could correspond to the 5F5 → 5I8 and (5S2, 5F4) → 5I8 transitions of Ho3+, respectively . It can be seen that the intensity of the up-conversion fluorescence is the largest when the molar ratio of Ho3+ and Yb3+ is 1:4. Figure 1b presents the up-conversion photofluorescence of Ho3+-Yb3+-Mg2+ tri-doped TiO2 with different doping contents of Mg2+ (Ho:Yb:Mg:Ti = 1:4:x:100, molar ratio). The up-conversion fluorescence was enhanced by the addition of Mg2+. When the doping content of Ho3+:Yb3+:Mg2+ = 1:4:2, the up-conversion emission is the strongest for Ho3+-Yb3+-Mg2+ tri-doped TiO2. Hereinafter, the UC-Mg-TiO2 with the molar ratio of Ho3+:Yb3+:Mg2+:Ti = 1:4:2:100 was applied.
Figure 2 shows the X-ray diffraction of TiO2 (30NR-D) and UC-Mg-TiO2. According to the PDF card (JCPDS card no.21–1272), the peaks located at 2θ = 25.6 °, 37.7 °, 48.1 °, and 53.7 ° in the patterns could belong to the (101), (004), (200), (105), (211), and (204) crystal planes, respectively. This displays the phase of UC-Mg-TiO2 is anatase.
To demonstrate the doping of Ho, Yb, and Mg into TiO2, the X-ray photoelectron spectra of UC-Mg-TiO2 were obtained. The XPS survey spectrum of UC-Mg-TiO2 was presented in Additional file 1: Figure S2. Figure 3a shows the high-resolution photoelectron peaks of Ti 2p, which had two peaks of Ti 2p1/2 and Ti 2p3/2 located at 463.7 eV and 458.2 eV, respectively. Figure 3b, c shows the high-resolution photoelectron peaks of Ho 4d and Yb 4d, which appear at 163.6 eV and 192.3 eV, respectively. These agree with the reported peak positions . Figure 3d presents the photoelectron peak of Mg 2p located at 49.8 eV . These data displays that Ho, Yb, and Mg atoms were incorporated into TiO2.
Figure 4a shows the absorption spectra of TiO2 (30NR-D) and UC-Mg-TiO2. There are five absorption peaks appear in the absorption spectrum of UC-Mg-TiO2, which are corresponding to characteristic absorption of Ho3+ and Yb3+. It can be seen that the doping of Ho, Yb, and Mg improves the absorption of TiO2 in visible light region and expands its absorption to NIR range. The Tauc plot can be used to estimate the energy band gap of material . The Tauc plots from the absorption spectra were presented in Fig. 4b. The energy band gap values can be calculated to be 3.09 eV and 3.18 eV for UC-Mg-TiO2 and TiO2 (30NR-D), respectively. The UC-Mg-TiO2 presents a smaller band gap than TiO2.
Figure 5 shows the SEM photograph of TiO2 (30NR-D) and UC-Mg-TiO2 films. The size of the nanoparticle is about 25 nm for 30 NR-D, and particle size is about 28 nm for UC-Mg-TiO2. The two films are uniform. Thus, the UC-Mg-TiO2 displays a similar morphology and particle size to TiO2 (30NR-D).
The PSCs were fabricated based on the electron transfer layers with and without UC-Mg-TiO2. The electron transfer layer with UC-Mg-TiO2 was prepared by spin-coating the mixed solution of UC-Mg-TiO2 sol and TiO2 sol (UC-Mg-TiO2:TiO2 = x:(100 − x), x = 0, 20, 40, 60, 80, and 100, v/v). I-V measurements of the solar cells were performed, and from which the photovoltaic parameters were abstracted. The Isc, Voc, FF, and PCE of the solar cells in this work were obtained by an average of the values of 20 samples. The relation of PCE with the contents of UC-Mg-TiO2 was displayed in Fig. 6a. Firstly, the PCE of the solar cells becomes large, and after that becomes small with the increase of the UC-Mg-TiO2 contents, which reaches the maximum value at the content of 60% (UC-Mg-TiO2:TiO2 = 60:40, v/v). Table 1 presents the photovoltaic parameters of solar cells based on the electron transfer layers with and without UC-Mg-TiO2. The open-circuit voltage (Voc) and short-circuit current (Isc) of the solar cells with UC-Mg-TiO2 were increased to 1.05 V and 22.6 mA/cm2 from 1.03 V and 21.2 mA/cm2 for the solar cells without UC-Mg-TiO2, respectively. Thus, the PCE of the devices based on the electron transfer layer with UC-Mg-TiO2 was improved to 16.3% from 15.2% for those without UC-Mg-TiO2. The typical I-V curves of the devices are shown in Fig. 6b. The PCE histograms of the solar cell performance of 20 samples with and without UC-Mg-TiO2 are presented in Additional file 1: Figure S3.
Some experiments were carried out to explain the improvement. Figure 7 displays the energy band structures of the materials contained in the solar cells based on some reports [25, 26], and the energy band gap from the Tauc plots is shown in Fig. 4b. The conduction band difference between perovskite and TiO2 becomes larger for UC-Mg-TiO2 compared with that of TiO2 (30NR-D), since the UC-Mg-TiO2 has a smaller band gap than TiO2 (30NR-D). This may be one of the reasons to give a larger Voc for the devices based on the electron transfer layer with UC-Mg-TiO2 [27, 28].
Figure 8a shows the steady-state photoluminescence (PL) of the perovskite films on the electron transfer layers with and without UC-Mg-TiO2. The PL peak located at 760 nm is originated from the perovskite film . The PL intensity of the perovskite film on electron transfer layer with UC-Mg-TiO2 decreased compared with that of perovskite film on electron transfer layer without UC-Mg-TiO2. This implies that the electron transport and extraction of UC-Mg-TiO2 from the perovskite film is more efficient than that of TiO2 (30NR-D). This can be further demonstrated by the time-resolved photoluminescence (TRPL) of the samples shown in Fig. 8b. It can be seen that the decay time of TRPL for the perovskite film on electron transfer layer with UC-Mg-TiO2 is faster than that of perovskite film on electron transfer layer without UC-Mg-TiO2. This indicates that the charge transfer for the former is faster than the latter [30, 31].
Figure 9a shows the Nyquist plots obtained from the electrochemical impedance spectroscopy (EIS) of the solar cells based on the electron transfer layer with and without UC-Mg-TiO2. The Nyquist plots can be fitted by an equivalent circuit which is schematically shown in Fig. 9b. The Rs, Rrec, and Cμ are the series resistance, recombination resistance, and the capacitance of the device [32, 33]. The detailed fitting values are presented in Table 2. The Rs value of the devices based on the electron transfer layers with UC-Mg-TiO2 is nearly the same with that of those without UC-Mg-TiO2. While the Rrec value of the devices based on electron transfer layer with UC-Mg-TiO2 is larger than that of those without UC-Mg-TiO2. This implies that UC-Mg-TiO2 could effectively decrease the change recombination.
To confirm the contributions of the up-conversion material UC-Mg-TiO2 to the photocurrent of the solar cells, the I-V measurements were carried out under the simulated solar radiation filtered with a band-pass NIR filter (980 ± 10 nm). Figure 10a displays the I-V curves of the solar cells based on the electron transfer layers with and without UC-Mg-TiO2. The short-circuit current (Isc) of the solar cells with UC-Mg-TiO2 is obviously larger than that of those without UC-Mg-TiO2. This demonstrates the effect of UC-Mg-TiO2 on the photocurrent of the solar cells, because UC-Mg-TiO2 converts the near-infrared photons into visible photons, which the solar cells can absorb to produce additional photocurrent [7, 17]. Figure 10b shows the IPCE spectra of the solar cells with and without UC-Mg-TiO2. The IPCE of the solar cells with UC-Mg-TiO2 is increased, especially at the range of 400~650 nm, compared with that of those without UC-Mg-TiO2. This could be caused by the up-conversion effect of UC-Mg-TiO2 [7, 17].
The up-conversion nanomaterial of Ho3+-Yb3+-Mg2+ tri-doped TiO2 (UC-Mg-TiO2) was synthesized successfully. The up-conversion emissions of the UC-Mg-TiO2 were enhanced with an addition of Mg2+. We applied the UC-Mg-TiO2 to the PSCs, in which the UC-Mg-TiO2 was used to modify the electron transfer layer. The Voc and Isc of the devices with UC-Mg-TiO2 were improved to 1.05 V and 22.6 mA/cm2 from 1.03 V and 21.2 mA/cm2 for those without UC-Mg-TiO2, respectively. And the PCE of the devices with UC-Mg-TiO2 was increased to 16.3% from 15.2% for those without UC-Mg-TiO2.
Electrochemical impedance spectroscopy
Power conversion efficiency
Perovskite solar cells
Yang WS, Noh JH, Jeon NJ, Kim YC, Ryu S, Seo J, Seok SI (2015) High-performance photovoltaic perovskite layers fabricated through intramolecular exchange. Science 348:1234–1237
Wang YF, Wu J, Zhang P, Liu DT, Zhang T, Ji L, Gu XL, Chen ZD, Li SB (2017) Stitching triple cation perovskite by a mixed anti-solvent process for high performance perovskite solar cells. Nano Energy 39:616–625
Li SB, Zhang P, Wang YF, Sarvari H, Liu DT, Wu J, Yang YJ, Wang ZM, Chen ZD (2017) Interface engineering of high efficiency perovskite solar cells based on ZnO nanorods using atomic layer deposition. Nano Res 10:1092–1103
Yang WS, Park BW, Jung EH, Jeon NJ, Kim YC, Lee DC, Shin SS, Seo J, Kim EK, Noh JH, Seok SI (2017) Iodide management in formamidinium lead halide based perovskite layers for efficient solar cells. Science 356:1376–1379
Zhang T, Wu J, Zhang P, Ahmad W, Wang YF, Alqahtani M, Chen H, Gao CM, Chen ZD, Wang ZM, Li SB (2018) High speed and stable solution-processed triple cation perovskite photodetectors. Adv Optical Mater 6:1701341
Jeon NJ, Na H, Jung EH, Yang TY, Lee YG, Kim G, Shin HW, Seok SI, Lee J (2018) A fluorene-terminated hole-transporting material for highly efficient and stable perovskite solar cells. Nature Energy. https://doi.org/10.1038/s41560-018-0200-6
He M, Pang XC, Liu XQ, Jiang BB, He YJ, Snaith H, Lin ZQ (2016) Monodisperse dual-functional upconversion nanoparticles enabled near-infrared organolead halide perovskite solar cells. Angew Chem Int Ed 55:4280–4284
Roh JM, Yu HJ, Jang J (2016) Hexagonal β-NaYF4:Yb3+, Er3+ nanoprism incorporated upconverting layer in perovskite solar cells for near-infrared sunlight harvesting. ACS Appl Mater Interfaces 8:19847–19852
Zhang P, Li SB, Liu CH, Wei XB, Wu ZM, Jiang YD, Chen Z (2014) Near-infrared optical absorption enhanced in black silicon via Ag nanoparticle-induced localized surface plasmon. Nanoscale Res Lett 9:519–523
Yu J, Yang YL, Fan RQ, Zhang HJ, Li L, Wei LG, Shi Y, Pan K, Fu HG (2013) Er3+ and Yb3+ co-doped TiO2-xFx up-conversion luminescence powder as a light scattering layer with enhanced performance in dye sensitized solar cells. J Power Sources 243:436–443
You S, Wang H, Bi SQ, Zhou JY, Qin L, Qiu XH, Zhao ZQ, Xu Y, Zhang Y, Shi XH, Zhou HQ, Tang ZY (2018) A biopolymer heparin sodium interlayer anchoring TiO2 and MAPbI3 enhances trap passivation and device stability in perovskite solar cells. Adv Mater 30:1706924
Kim W, Park J, Kim H, Pak Y, Lee H, Jung GY (2017) Sequential dip-spin coating method: fully infiltration of MAPbI3-xClx into mesoporous TiO2 for stable hybrid perovskite solar cells. Electrochemi Acta 245:734–741
Choi J, Song S, Horantner MT, Snaith HJ, Park T (2016) Well-defined nanostructured, single crystalline TiO2 electron transport layer for efficient planar perovskite solar cells. ASC Nano 10:6029–6036
Giordano F, Abate A, Baena JPC, Saliba M, Matsui T, Im SH, Zakeeruddin SM, Nazeeruddin MK, Hagfeldt A, Graetzel M (2016) Enhanced electronic properties in mesoporous TiO2 via lithium doping for high-efficiency perovskite solar cells. Nat Commun 7:10379
Liu JW, Zhang J, Yue GQ, Lu XW, Hu ZY, Zhu YJ (2016) W-doped TiO2 photoanode for high performance perovskite solar cell. Electrochimi Acta 195:143–149
Wu MC, Chan SH, Jao MH, Su WF (2016) Enhanced short-circuit current density of perovskite solar cells using Zn-doped TiO2 as electron transport layer. Sol Energ Mater Sol C 157:447–453
Yu J, Yang Y, Fan R, Liu DQ, Wei LG, Chen S, Li L, Yang B, Cao WW (2014) Enhanced near-infrared to visible upconversion nanoparticles of Ho3+-Yb3+-F− tri-doped TiO2 and its application in dye-sensitized solar cells with 37% improvement in power conversion efficiency. Inorg Chem 53:8045–8053
Zhang HY, Shi JJ, Xu X, Zhu LF, Luo YH, Li DM, Meng QB (2016) Mg-doped TiO2 boosts the efficiency of planar perovskite solar cells to exceed 19%. J Mater Chem A 4:16383–16389
He YY, Wu JL, Wang XH, Feng ZQ, Dong B (2016) Optical temperature sensing behavior through stark sublevels transitions of green and red upconversion emissions for Er3+-Yb3+-Li+ codoped TiO2 phosphors. J Nanosci Nanotechnol 16:3768–3771
Michael S, Taisuke M, Seo JY, Domanski K, Correa-Baena JP, Nazeeruddin MK, Zakeeruddin SM, Tress W, Abate A, Hagfeldtd A, Gratzel M (2016) Cesium-containing triple cation perovskite solar cells: improved stability, reproducibility and high efficiency. Energy Environ Sci 9:1989–1997
Huang X, Han S, Huang W, Liu X (2013) Enhancing solar cell efficiency: the search for luminescent materials as spectral converters. Chem Soc Rev 42:173–201
Mazierski P, Lisowski W, Grzyb T, Winiarski MJ, Klimczuk T, Mikolajczyk A, Flisikowski J, Hirsch A, Kolakowska A, Puzyn T, Zaleska-Medynska A, Nadolna J (2017) Enhanced photocatalytic properties of lanthanide-TiO2 nanotubes: an experimental and theoretical study. Appl Catalysis B 205:376–385
Cheng G, Akhtar MS, Yang OB, Stadler FJ (2016) Nanoprecursor-mediated synthesis of Mg2+-doped TiO2 nanoparticles and their application for dye-sensitized solar cells. J Nanosci Nanotechno 16:744–752
Gao XX, Ge QQ, Xue DJ, Ding J, Ma JY, Chen YX, Zhang B, Feng YQ, Wan LJ, Hu JS (2016) Tuning the fermi-level of TiO2 mesoporous layer by lanthanum doping towards efficient perovskite solar cells. Nanoscale 8:16881–16885
Chen H, Yang B, Shuang X, Zhang T, Meng XY, Ng WK, Yang YL, Wong KS, Chen HN, Yang SH (2017) Tuning the A-site cation composition of FA perovskites for efficient and stable NiO-based p-i-n perovskite solar cells. J Mater Chem A 5:21858–21865
Rhee JH, Chung CC, Diau WG (2013) A perspective of mesoscopic solar cells based on metal chalcogenide quantum dots and organometal-halide perovskites. NPG Asia Mater 5:e68
Li YL, Sun WH, Yan WB, Ye SY, Peng HT, Liu ZW, Bian ZQ, Huang CH (2015) High-performance planar solar cells based on CH3NH3PbI3-xClx perovskites with determined chlorine mole fraction. Adv Funct Mater 25:4867–4873
Kim HS, Park NG (2014) Parameters affecting I-V hysteresis of CH3NH3PbI3 perovskite solar cells: effects of perovskite crystal size and mesoporous TiO2 layer. J Phys Chem Lett 5:2927–2934
Grancini G, Roldán-Carmona C, Zimmermann I, Mosconi E, Lee X, Martineau D, Narbey S, Oswald F, De Angelis F, Graetzel M, Nazeeruddina MK (2017) One-year stable perovskite solar cells by 2D/3D interface engineering. Nat Commun 8:15684
Zhao L, Luo D, Wu J, Hu Q, Zhang W, Chen K, Liu T, Liu Y, Zhang Y, Liu F, Russell TP, Snaith HJ, Zhu R, Gong Q (2016) High-performance inverted planar heterojunction perovskite solar cells based on lead acetate precursor with efficiency exceeding 18. Adv Funct Mater 26:3508–3514
Zhou H, Chen Q, Li G, Luo S, Song TB, Duan HS, Hong Z, You J, Liu Y, Yang Y (2014) Interface engineering of highly efficient perovskite solar cells. Science 345:542–546
Huang Y, Zhu J, Ding Y, Chen S, Zhang C, Dai S (2016) TiO2 sub-microsphere film as scaffold layer for efficient perovskite solar cells. ACS Appl Mater Inter 8:8162–8167
Yun J, Ryu J, Lee J, Yu H, Jang J (2016) SiO2/TiO2 based hollow nanostructures as scaffold layers and Al-doping in the electron transfer layer for efficient perovskite solar cells. J Mater Chem A 4:1306–1311
This work is supported by the NSFC-Henan Province Joint Fund (U1604144), Program for Science and Technology Innovation Talents in Universities of Henan Province (no.16HASTIT043), Science Fund of Henan Province (162300410020), Science Project of Education Department of Henan Province (no.17A140005), Foundation for Young Key Teacher by Henan Province (no. 2014GGJS-135), and Science and Technology Development Project of Henan Province (no.172102410043).
Availability of Data and Materials
All data are fully available without restriction.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Figure S1. Up-conversion mechanisms of the Ho3+-Yb3+ co-doped TiO2. Figure S2. XPS survey of UC TiO2. Figure S3 PCE histograms of the solar cell performance of 20 samples with and without UC-Mg-TiO2. (DOCX 77 kb)